60 5. Macroscopic measurements in Cr7Ni and Cr8Ni

Figure 20: Schematic view of Cr_{8}Ni compound.

well-known Cr_{8} ring and the spin segments Cr_{8}Zn, Cr_{8}Cd have been taken into account,
where Zn^{2+} and Cd^{2+} are two non magnetic ions. If the ion inserted in the ring-shape
structure is magnetic, an AF ring with an odd number N of magnetic ions is obtained.

In the case of odd-membered AF rings, magnetic properties are expected to be changed
drastically due to the spin frustration effects. The simplest AF ring with N odd is a
sys-tem with three spins s=1/2 antiferromagnetically coupled: within this regard V_{15} [69]

and Cu_{3} [70] molecular magnets are good examples. In these frustrated triangular AF
spin systems the ground state is a magnetic S = 1/2 [69]. Other odd-membered AF
rings with N >3 have been more difficult to synthesize. Quite recently a new family
of odd-membered AF rings with N =9 has been created with the synthesis of a
het-erometallic Cr-based ring-shaped AF magnet (C_{6}H_{11})_{2}NH_{2}[Cr_{8}NiF_{9}(O_{2}CC(CH_{3})_{3})_{18}]
(in short, Cr_{8}Ni) by Winpenny and co-workers [66,71,72]. The Cr_{8}Ni is the first
odd-membered AF ring with N >3. The cluster shows spin frustration effects because
all antiferromagnetic interactions can not be simultaneously satisfied. For this reason,
Cr8Ni molecule can be regarded as a magnetic analogue of the M¨obius strip [66,71]. Due
to the odd number of spins it is impossible to align all nearest neighbour spins
antipar-allel to each other. The region where the spins are not antiparantipar-allel can be considered
as a knot of the M¨obius strip. The precursor of Cr_{8}Ni is a well known even membered
AF ring [Cr_{8}F_{8}(O_{2}CC(CH_{3})_{3})_{16}]0.25C_{6}H_{14} (in short, Cr_{8}) whose ground state is spin
singlet S=0 state due to AF interaction (J_{Cr−Cr} ≈16.9 K) between nearest neighbor
Cr^{3+} (s=3/2) spins [39]. The Cr8Ni is basically obtained by inserting a Ni^{2+} (s=1) ion
into the Cr_{8} ring. The metal ions are bridged by one fluoride and two (CH_{3})3CCO_{2}
radicals [66,71]. The antiferromagnetic interactions between Cr^{3+} ions and between
Cr^{3+} and Ni^{2+} ions are reported to be J_{Cr−Cr}=16 K and J_{Cr−N i}=70 K respectively.

5.2. The Cr8Ni heterometallic ring 61

1 1 0 1 0 0

0 . 0 0 0 . 0 4 0 . 0 8 0 . 1 2 0 . 1 6 0 . 2 0

e x p c a l c u l a t i o n

χ(emu/mol)

T ( K )

Figure 21: Measured (scatters) and calculated (line) temperature dependence of mag-netic susceptibility chi in Cr8Ni. The fall of χ at T ≈0 strongly support the occurence of a non magnetic ground state. Experimental data are taken from Ref. [66].

These values were obtained by a fit of the temperature dependence of the magnetic susceptibility χ which shows two peaks around 2K and 25K (see Fig. 21) [66,71]. From the fitting of the magnetic susceptibility in the temperature range T =1.6-300 K it is also inferred that the ground state is a singlet S = 0 and that the first excited state is a S = 1 at 3.7 K from the ground state. This fit was based on a spin Hamiltonian with only the isotropic Heisenberg exchange term. The presence of a singlet ground state in this frustrated ring is quite interesting and requires more direct experimental evidence.

In order to obtain more information on the ground state of the Cr_{8}Ni system from an
experimental point of view, it is important to investigate the magnetic properties at
low temperature, i.e. well below the lowest energy gap temperature. However, there
are no experimental studies of magnetic properties on this cluster at low temperatures
below 1 K up to now. The magnetization and NMR experiments performed on Cr_{8}Ni
clearly show evidence of a spin singlet ground state and allows to establish the energy
separation of the low-lying quantum magnetic states. The experimental results are in
good agreement with predictions from theoretical calculations. Interestingly, the width
of the steps in the field-dependence of the magnetization and the lack of sharp minima
in the field-dependence of the specific heat show that sizeable Dzyaloshinski-Moriya
(DM) interactions are present and lead to anticrossings between states of different
to-tal spin.

Fig. 22(a) shows the magnetization curves for Cr_{8}Ni at T =0.1 K for increasing
(de-creasing) magnetic fields: a clear step-wise increase (decrease) of magnetization is
observed. The magnetization curves are nearly the same with no striking hysteresis

62 5. Macroscopic measurements in Cr7Ni and Cr8Ni

02468

1 0

0 5 1 0 1 5 2 0 2 5 3 0

0123456M (µ B/f.u.)

i n c r e a s i n g f i e l d d e c r e a s i n g f i e l d M t o t

### ( a )

### ( b )

dM/dH (a.u.)

M a g n e t i c F i e l d ( T )

Figure 22: Magnetization curve of Cr8Ni measured at T =0.1 K. Blue line shows the
theoretical calculated results for T =0.1 K with the following parameters: J_{Cr−Cr}=14.7
K, J Cr− Ni=85 K, dCr=-0.42 K and d_{N i}=-4.9 K. (b) dM/dH curve at T =0.1 K.

Blue line shows the theoretical calculated results for T =0.1 K.

for the up and down magnetic process at this temperature. The magnetization rapidly
increases step by step with plateaus at≈ 2µB,≈ 4µB,≈ 6µB,≈ 8µB,≈ 10µB between
the transition fields H_{n} (n=1,2,...). The H_{n} is determined by the peak positions of
dM/dH curves [see Fig. 22(a)] to be 2.81, 12.8, 18.3, 23.5, and 28.5T, for n=1, 2,
3, 4, and 5, respectively. Line width (δH) defined at half amplitude for each peak in
dM/dH is estimated to be 3.07, 1.61, 1.69, 2.15, and 2.06 T for n=1, 2, 3, 4, and 5,
respectively. These values are larger than an expected thermal width 0.26 T for T=0.1
K estimated from an equation of δH = 3.53k_{B}T /gµ_{B} with an assumption of g ≈ 2. As
discussed below, the broadening is also too large to be attributed merely to the
distri-bution of level crossing fields Hn in the powder sample, and it is thus an indication of
the presence of level anticrossing effects. If the ground state of system were magnetic,
one should observe Brillouin function-like increase for the initial magnetization. The
observed convex downward magnetization curve clearly proves a nonmagnetic ground

5.2. The Cr8Ni heterometallic ring 63

0 1 2 3 4 5 6

048

1 2

∆H (T) n

e x p e r i m e n t t h e o r y

Figure 23: H-dependence of ∆H. Closed and open symbols show experimental and theoretical results respectively.

state. Thus the H_{n} are the level crossing fields between the S=0 ground state and the
first excited S=1 for n=1, between S=1 and S=2 for n=2 and so on. The difference
between adiacent level crossing fields defined as ∆H = H_{n}− Hn−1 (where H_{0} is zero)
as a function of n is shown in Fig. 23. The n-dependence of ∆H for Cr8Ni does not
follows the Land´e’s rule which predicts that ∆H is independent of n. Fig. 24 shows
the H-dependence of the specific heat C_{total} at T =0.5 K while the inset shows the
temperature dependence of the specific heat C_{total}under zero magnetic field. The
mea-sured specific heat is the sum of a magnetic contribution and a lattice contribution, i.e.

C_{total} = C_{mag}+ C_{lattice}. However, as we will discuss later, the observed specific heat at
T =0.5 K can be considered mainly due to the magnetic contributions Cmag. A single
broad peak is observed around the first level crossing H_{1}=2.82 T. At the second level
crossing, one can resolve two peaks at 12.1 and 13.7 T with a small dip around 13.0 T.

In presence of a level crossing one should indeed observe two peaks with a dip in the
middle. This is due to a Schottky-type anomaly as it was observed in even membered
AF rings Fe_{6} [73] and Cr_{8} [63]. The two-level Schottky model predicts

C_{s} = (∆(H)/k_{B}T )^{2}× exp(∆(H)/kBT )/(1 + exp(∆(H)/k_{B}T ))^{2}

a behavior which yields a maximum when ∆(H) ≈2.5 kBT . Near a level crossing
field, the energy separation ∆(H) between two lowest-lying states can be expressed
approximately as ∆(H) ≈ gµB|Hn− H| and thus two maxima are expected at |H −
H_{n}|=2.5 kBT /gµ_{B}with a dip at H_{n}where ∆(H) is smallest. In presence of a pure level
crossing the dip between the two Schottky-like peaks should go down to zero since at
level crossing ∆(H)=0 while in presence of a level repulsion (level anticrossing) the dip

64 5. Macroscopic measurements in Cr7Ni and Cr8Ni

0 . 1 1 1 0 1 0 0

0 . 0 1 0 . 1

1

1 0 1 0 0

0 2 4 6 8 1 0 1 2 1 4

0 . 0 0 . 2 0 . 4 0 . 6 0 . 8 1 . 0

C/R

T ( K ) e x p C t o t a l/ R C l a t t i c e/ R H = 0

e x p w i t h o u t D M w i t h D M

C/R

M a g n e t i c F i e l d ( T ) T = 0 . 5 K

Figure 24: H-dependence of the specific heat at T =0.5 K. Solid line is theoretical
calculated results for T =0.5K. The inset shows temperature dependence of specific heat
measured under zero magnetic field. Red and broken lines in the inset show calculated
C_{total} and C_{lattice}, respectively. C_{lattice} is calculated from the Eq. (82) with this set of
parameters: r=343, Θ_{D}=180 K and d=0.27

can be much less pronounced and it gives a measure of the gap at the anticrossing [63].

As shown in Fig. 24a small dip superimposed on a broad maximum is observed only at the second level crossing. The broadening of the peaks cannot be ascribed to the distribution of the level crossing fields in a powder sample as will be demonstrated below in the discussion of the broadening of the magnetization steps. Thus one can conclude that at both the first and second level crossing a sizeable gap exists between the two crossing levels (level anticrossing).

The spin singlet ground state in Cr8Ni is also revealed by proton NMR spectrum
measurements at H=0.2 T. We observed a single narrow line of ^{1}H-NMR as shown in
the inset of Fig. 25. The full width at half amplitude (FWHA) decreases from ≈62
kHz (≈15 Oe) at T =1 K on lowering temperature and becomes almost independent of
T (≈42 kHz (≈10 Oe)) below ≈0.6 K as shown in Fig. 25. The FWHA≈10 Oe can
be explained by nuclear-nuclear dipolar interactions. In fact the nuclear dipolar field
between two protons is of the order of γn~/r^{3} ≈8.3 Oe when one assumes an internuclear
distance r = 1.5 ˚A (γ_{n} is the gyro magnetic ratio of a proton). Thus we may conclude
there is no magnetic broadening in the spectrum due to the Cr and/or Ni spin moments.

This is consistent with a total spin S=0 ground state and also with a zero expectation

5.2. The Cr8Ni heterometallic ring 65

0 . 0 0 . 5 1 . 0 1 . 5 2 . 0 2 . 5

0 . 0 4 0 . 0 6 0 . 0 8 0 . 1 0 0 . 1 2

8 . 3 8 . 4 8 . 5 8 . 6 8 . 7

FWHA ( MHz )

T ( K )

C r 8 N i ( H = 0 . 2 T ) C r 8 C d ( H = 0 . 1 9 T )

f ( M H z ) T = 0 . 1 K

Figure 25: Temperature dependence of full width of half amplitude (FWHA) of ^{1}
H-NMR spectra in Cr8Ni (closed circles) at H=0.2 and Cr8Cd (closed squares) at H=0.19
T. The inset shows a typical ^{1}H-NMR spectrum in Cr_{8}Ni at T =0.1K

value for the local spin component at each ion site. To check this conclusion, we have
measured the FWHA of^{1}H-NMR spectrum at nearly the same magnetic field H=0.19 T
in a similar odd membered Cr-based AF ring Me_{2}NH_{2}[Cr_{8}CdF_{9}(O_{2}CCMe_{3})_{18}] (in short,
Cr_{8}Cd) which has a spin singlet ground state with a first excited spin triplet state at∼3
K above the ground state [7,52]. As shown in Fig. 25, the FWHA for both compounds
coincide at low temperatures within our experimental uncertainty, indicating that the
FWHA of about 10 Oe originates from the nuclear dipolar interaction, which is the same
for isostructural Cr_{8}Ni and Cr_{8}Cd. We turn now to a quantitative comparison of the
experimental results with the theoretical calculations. The starting spin Hamiltonian
for the odd membered AF ring is

H = J_{Cr−N i}(S_{8}· SN i+ S_{N i}· S1) + J_{Cr−Cr}

7

X

i=1

S(i)· S(j)

+d_{Cr}

8

X

i=1

S_{z}^{2}(i)− SCr(S_{Cr}+ 1)/3 + dN iS_{z,N i}^{2} − SN i(S_{N i}+ 1)/3

−gCrµ_{B}

8

X

i=1

H· Si− gN iµ_{B}H· SN i, (80)

where i labels the eight Cr ions (spins). The first and second terms describe the dominant isotropic Heisenberg interaction. Here we assume two differente exchange costants, one between Cr and Ni spins (JCr−N i) and another between Cr spins (JCr−Cr).

The third and fourth terms describe local crystal fields, where d_{Cr} and d_{N i} represent
the uniaxial single ion anisotropy for Cr and Ni ions, respectively. Finally, the fifth
and sixth terms represent the Zeeman interactions. The two exchange parameters

66 5. Macroscopic measurements in Cr7Ni and Cr8Ni

have been determined to be J_{Cr−Cr}=14.7 K and J_{Cr−N i}=85 K by fitting magnetization
and susceptibility data. Reasonable values of d_{Cr} an d_{N i} turn out to produce tiny
effects in the powder properties. Hence we assume d_{Cr}=-0.42 K as in the parent Cr_{8}Zn
compound [8] and the same ratio of d_{Cr} to d_{N i} as in Cr_{7}Ni [68], yielding d_{N i} =-4.9 K.

The Hamiltonian is diagonalized by following the procedure described in Ref. [39]. The
calculated eigenstates and eigenvalues have been used to evaluate the H-dependence
of the thermal averaged magnetization and specific heat (C_{mag}) as well as the T
-dependence of χ and C_{mag}. Since we used polycrystalline samples, all calculated results
are powder averaged so that they can be directly compared with the experimental
observations. By using g_{Cr}=1.98 and g_{N i}=2.2, the T -dependence of χ (see the solid
line in the Fig. 21) and the positions of the observed values of H_{n} are well reproduced
[see Fig. 23(c)]. The n dependence of ∆H is also well reproduced by the theory as
shown in Fig. 23. On the other hand, the width of the calculated peaks is much smaller
than the experimental results as shown in Fig. 22(b). The origin of the broadening
of the magnetization steps is likely to be the same as the origin of the broadening
of the specific heat peaks and is discussed after the presentation of the specific heat
results. The temperature dependence of the calculated specific heat C is shown by a
line in the inset of Fig. 24. The temperature dependence of the calculated specific heat
C_{total}(= C_{mag}+ C_{lattice}) is shown by a red solid line in the inset of Fig. 24. C_{mag} was
calculated from the following equation [39]:

C_{mag}
Rβ^{2}

P

iE_{i}^{2}exp(−βEi)P

iexp(−βEi)− [Eiexp(−βEi)]

[P

iexp(−βEi)] , (81)

where E_{i} are the eigenvalues obtained from Eq. (80), and β = (k_{B}T )^{−1}. The lattice
contribution to C has been estimated from a phenomenological model [74];

C_{lattice}/R = 234rT^{3}/(Θ_{D}+ δT^{2})^{3} (82)

where r is the number of atoms per molecule, and Θ_{D} and δ are parameters. For Cr_{8}Ni,
we used a set of parameters: r=343, ∆_{D}=180 K and δ =0.27 whose values are very
similar to those reported for the isostructural AF ring Cr_{8}Cd [52]. The broken line in
the inset shows the calculated C_{lattice}. The specific heat at low temperatures (below 1
K) is dominated by the magnetic contribution (Cmag). The result is in good agreement
with the experimental data as in the inset of Fig. 24. It should be noted that we did
not use any scaling factors to fit the experimental data by the calculation. On the
other hand the calculated C_{mag} at T =0.5 K as a function of H, shown by a dashed line

5.2. The Cr8Ni heterometallic ring 67

in Fig. 24, is not in good agreement with the experiments. The problem is the remark-able broadening of the peak in the experimental specific heat at level crossings, which should have the same origin as the broadening in the magnetization steps [see Fig.

22(a)] and which is not reproduced by calculations based only on Eq. (80). We have
already introduced reasonable single-ion terms in the calculations, hence the
broaden-ing effects in the experiment cannot be simply attributed to a distribution of Hn due
to the random direction of crystal-field anisotropy axes in a powder sample. In
prin-ciple, a distribution of exchange parameters from molecule to molecule resulting from
disorder (J -strain) might produce a broadening. For instance, in Cr_{7}Ni, a distribution
with standard deviation of the order of 2.5% was found [68]. However we find that an
unrealistically large value for the standard deviation has to be assumed to account for
the entity of the observed effects. In addition, the effect of J -strain on the minimum in
C at 2.7 T is much smaller than that on the minimum at 13 T, whereas in experimental
data the broadening is of the same entity in the two minima. On the other hand, if the
level crossings (LCs) are not true crossings but level anticrossings(ACs), C_{mag} does not
vanish at H_{n} because ∆(H) remains finite. By considering only the lowest multiplet
for each value of S, even-S and odd-S multiplets belong to different irreducible
rep-resentations of the ideal spin permutational symmetry of Eq. (80). Hence, crossings
can be turned into ACs only by including in the Hamiltonian terms which break this
symmetry (for instance site-dependent Cr crystal fields). However, this sort of
sym-metry lowering would not significantly affect the first crossing at 2.7 T. In fact, only
a DM interaction can directly mix the S=0 and S=1 multiplets because it is the only
term (beside the Zeeman term which does not break spin permutational symmetry)
which is described by rank-one complex tensor operators T_{Q}^{1} and because if K > 1
S = 0

T_{Q}^{K}

S = 1 = 0. Hence, the absence of a minimum in C(H) at 2.7 T provides strong evidence of the presence of DM interactions in the microscopic Hamiltonian.

The most likely sources of this interaction are the two Cr-Ni bonds because the
inver-sion symmetry is maximally broken and the exchange interaction is the strongest. In
addition, the orbital degrees of freedom which are besides the DM interaction are much
less quenched in Ni^{2+} than in Cr^{3+} ions. To investigate the effect of DM interactions,
we have made calculations assuming the simplest possible choice for their form:

H_{DM} = D· (S8× SN i) + D· (SN i× S1) (83)
where we assume the two DM vectors to be equal and parallel to the z axis. The actual
DM vectors are very likely to be different than in Eq. (83), but our aim is not to look

68 5. Macroscopic measurements in Cr7Ni and Cr8Ni

0 2 4 6 8 1 0 1 2 1 4

05

1 0 1 5 2 0 2 5 3 0 3 5

05

1 0 1 5 2 0 2 5 3 0 3 5

M a g n e t i c F i e l d ( T )

Energy (K)Energy (K)

Figure 26: Magnetic-field dependence of the low-lying energy levels of Cr8Ni without (top) or with (bottom) DM interactions described by Eq. (83). The fields makes an angle of 45 degrees with the z axis. For each value of H the ground-state energy has been set to zero.

for a best fit of the data but merely to assess whether the DM interaction is a realistic
mechanism to explain the observed behavior or not. We assume for the modulus of
D the typical value D= 0.1 J_{Cr−N i}. The resulting spectrum is compared with that
obtained for D=0 in Fig. 26. Sizeable ACs open up at H_{n} whose amplitude depends
on the angle between the applied field and the z axis. The effect on C is shown by
the continuous line in Fig. 24. The DM interactions remove the sharp minima at Hn

in agreement with the experimental results. In addition, the width of steps in the calculated field-dependence of M is in very good agreement with experimental data [see the blue line in Figs. 22(a) and 22(b)]. Having established the main interactions appearing in the microscopic Hamiltonian we can study the properties of the resulting ground state for H = 0. Since isotropic exchange is the dominant interaction we focus on the ground state of the cluster Hamiltonian (80), neglecting crystal-field and DM interactions which do not qualitatively affect the ground state properties. While clas-sical calculations yield an infinite number of degenerate lowest-energy configurations, quantum mechanically the ground state is an S=0 singlet in agreement with

exper-5.2. The Cr8Ni heterometallic ring 69

1 2 3 4 5 6 7 8 9

- 3 . 5 - 3 . 0 - 2 . 5 - 2 . 0 - 1 . 5

0 1 2 3 4 5 6 7 8 9

- 3 - 2 - 1

01234

q u a n t u m c l a s s i c

**S** i**×****S** i-1 i

### ( a )

q u a n t u m c l a s s i c

**S** Ni**×****S** i i

### ( b )

Figure 27: Quantum and classic correlation functions nearest neighbours < Si· Si−1>

type in panel (a) (where i− 1 = 9 if i = 1) or < SN i· Si > type in panel (b).

imental observations. In order to investigate the structure of the ground state and,
in particular, how this is affected by frustration, we have used the following coupling
scheme |S18, S_{189}, S_{27}, S_{36}, S_{2736}, S_{45}, S_{273645}, S > [32] where S_{ijk}. . . are quantum
num-bers for the modulus of S_{i}+ S_{j}+ S_{k}+· + . . .. The Nickel ion is assumed to be in site 9.

We have found that the S=0 ground state (and the lowest multiplet for each value of S
up to S=11) is formed by states with S_{18}=3, S_{189}=2 for about the 95%. This indicates
that the Cr spins on sites 1 and 8 are practically locked antiparallel to the Ni spin and
parallel to each other.This originates from the much larger value of J_{Cr−N i}=85 K with
respect to J_{Cr−Cr}=14.7 K. Thus these three spins behave as an effective spin-2 degree
of freedom antiferromagnetically coupled to the two neighboring Cr spins. To
char-acterize the magnetic alignment of the spins in the ground state, we have calculated
static zero-temperature two-site correlations hSi· Sji and the corresponding quantities
for the classical Hamiltonian corresponding to Eq. (80). For the latter the spins are
classical vectors of length ps_{i}(s_{i}+ 1). We focus in particular on correlations of the
eight Cr spins with the Ni spin, shown in Fig. 27(a), and on nearest-neighbor
corre-lations shown in Fig. 27(b). Correlations < S_{N i}· S1 > and < S_{N i}· S8 > reflect the

70 5. Macroscopic measurements in Cr7Ni and Cr8Ni

Figure 28: This figure reports one of the degenerate configurations corresponding to
an S = 0 ground state calculated for the classical version of the model of Cr_{8}Ni. The
blue cone represents the Nickel ion. Within this reference frame, the angle between spin
4, 5 (whose bond is opposite to the Nickel site) and the spin of the Ni ion along z is

≈78^{◦}, while the angle between spin 4 and 5 is ≈156^{◦}, being z the axis perpendicular
to the plane of the ring. Therefore the knot is delocalized in the eight Cr ions with the
sites 4 and 5 having the same z component. The classic picture of the ground state
holds most of the main features of the quantum S = 0 ground state obtained from
exact diagonalization of the isotropic Heisenberg term in Eq. (80).

above-mentioned locking of the three spins in an S = 2 state. The meaning of the
remaining < S_{N i}· Si > correlations can be understood by inspecting the vector
struc-ture of the classical ground state (see Fig. 28), which shows a pattern of correlations
similar to that of the quantum ground state: classically, the spins are oriented in a
noncollinear fashion due to spin frustration. For instance, the Cr spins at sites 4 and
5 are almost lying in a plane perpendicular to the Ni spin which corresponds to nearly
vanishing correlations < S_{N i} · S4 > and < S_{N i} · S5 > as shown in Fig. 27(b). On
the other hand, quantum mechanically, the S=0 ground state approximately resonates
among the infinite classical configurations. Hence, local magnetic moments vanish at
low temperature due to quantum fluctuations, which is directly revealed by present
NMR measurements.